Silver Is Not Equal to Silver: Synthesis and Evaluation of Silver Nanoparticles with Low Biological Activity, and Their Incorporation into C12Alanine-Based Hydrogel

A new type of silver nanoparticles (AgNPs) was prepared and comprehensively studied. Scanning electron microscopy (SEM) and dynamic light scattering (DLS) analyses indicated that 24 nm AgNPs with narrow size distribution were obtained while Z-potential confirms their good stability. The composites of the obtained AgNPs with nontoxic-nature-inspired hydrogel were formed upon cooling of the aqueous solution AgNPs and C12Ala. The thermal gravimetric analysis (TGA) and the differential scanning calorimetry (DSC) do not show significant shifts in the characteristic temperature peaks for pure and silver-enriched gels, which indicates that AgNPs do not strongly interact with C12Ala fibers, which was also confirmed by SEM. Both AgNPs alone and in the assembly with the gelator C12Ala were almost biologically passive against bacteria, fungus, cancer, and nontumor human cells, as well as zebra-fish embryos. These studies proved that the new inactive AgNPs-doped hydrogels have potential for the application in therapy as drug delivery media.


Introduction
A huge challenge in modern medicine is the search for alternative and effective solutions to overcome the existing limitations in the diagnosis and treatment of various diseases. This applies mainly to cancer diseases, the treatment of which is associated with the problem of resistance to chemotherapy and with general toxicity of drugs for healthy tissues of the patient [1,2]. Another very important problem are bacterial and fungal infections, which are becoming more and more resistant to existing treatments. A promising idea is to use nanoparticles for this purpose as nanomedicines or delivery systems [3].
Nanotechnology is a field of science that has recently gained great interest in the scientific community due to the wide spectrum of applications in the food, electronics, and cosmetic industries, as well as medicine. The medical use of nanotechnology significantly supports the development of innovative methods of prevention, treatment, diagnosis, and in boiling aqueous solution by reduction of soluble silver salts by NaBH 4 or other mild reductant. The low-temperature syntheses are rare but they certainly may lead to AgNPs of a different structure and surface properties. This option was selected and the AgNPs were obtained at a room temperature in sodium citrate and tannic acid, physically purified, and dissolved in water to obtain a solution of 4.4 mg/mL concentration.
Physicochemical characteristics of AgNPs were determined using the DLS method, SEM, and ultraviolet-visible absorption spectroscopy (UV-Vis). Furthermore, the composition of the AgNPs surface was analyzed by means of X-ray photoelectron spectroscopy (XPS). The hydrodynamic diameter of obtained AgNPs, determined by DLS, was equal to 24 ± 5 nm with PDI (polydispersity index) of 0.04. The particle size and the PDI indicated the absence of aggregates in the tested suspension. The zeta potential of obtained nanoparticles, calculated to be −26 ± 6 mV, reveals high stability of the tested AgNPs suspension (at pH = 6.67), with a high negative surface charge resulting from the presence of dissociated citric acid molecules adsorbed on the surface of nanoparticles. The presence of a high surface charge effectively inhibits the process of aggregation of nanoparticles, which is observed in DLS (hydrodynamic diameter) analysis. The measurement results are shown in Figure 1.
growing seeds are concentration of reagents, reaction time, and also the temperature [32]. Each of these has a strong impact on morphological and physicochemical, as well as antibacterial, properties of the obtained nanomaterials. Typically, AgNPs are prepared in boiling aqueous solution by reduction of soluble silver salts by NaBH4 or other mild reductant. The low-temperature syntheses are rare but they certainly may lead to AgNPs of a different structure and surface properties. This option was selected and the AgNPs were obtained at a room temperature in sodium citrate and tannic acid, physically purified, and dissolved in water to obtain a solution of 4.4 mg/mL concentration.
Physicochemical characteristics of AgNPs were determined using the DLS method, SEM, and ultraviolet-visible absorption spectroscopy (UV-Vis). Furthermore, the composition of the AgNPs surface was analyzed by means of X-ray photoelectron spectroscopy (XPS). The hydrodynamic diameter of obtained AgNPs, determined by DLS, was equal to 24 ± 5 nm with PDI (polydispersity index) of 0.04. The particle size and the PDI indicated the absence of aggregates in the tested suspension. The zeta potential of obtained nanoparticles, calculated to be −26 ± 6 mV, reveals high stability of the tested AgNPs suspension (at pH = 6.67), with a high negative surface charge resulting from the presence of dissociated citric acid molecules adsorbed on the surface of nanoparticles. The presence of a high surface charge effectively inhibits the process of aggregation of nanoparticles, which is observed in DLS (hydrodynamic diameter) analysis. The measurement results are shown in Figure 1. The AgNPs monolayer for SEM observations was obtained by the diffusion-adsorption method [33] according to the random sequential adsorption (RSA) theory [34,35]. The AgNPs monolayer adsorbed on the polyethyleneimine (PEI)-modified silicon surface is shown in various magnifications in Figure 2a-c. The normalized Gauss distribution of diameters calculated by graphical analysis (ImageJ software) of SEM images is shown in Figure 2d. The average diameter of AgNPs determined by SEM is 31 nm. The difference in values of hydrodynamic diameter measured by the DLS and SEM methods is naturally explained by specificity of the techniques used [36]. The AgNPs monolayer for SEM observations was obtained by the diffusionadsorption method [33] according to the random sequential adsorption (RSA) theory [34,35]. The AgNPs monolayer adsorbed on the polyethyleneimine (PEI)-modified silicon surface is shown in various magnifications in Figure 2a-c. The normalized Gauss distribution of diameters calculated by graphical analysis (ImageJ software) of SEM images is shown in Figure 2d. The average diameter of AgNPs determined by SEM is 31 nm. The difference in values of hydrodynamic diameter measured by the DLS and SEM methods is naturally explained by specificity of the techniques used [36].
The electronic absorption spectra of the obtained AgNPs, as presented in Figure 3, show a characteristic intense narrow band at λ max = 400 nm and an additional band at λ max = 1000 nm. The stock solution of AgNPs with concentration of 1.9 mg/mL was used for preparation of more diluted solutions (20,40, and 60 µL of stock solution per 1 mL of water) for UV-Vis spectroscopy.  The electronic absorption spectra of the obtained AgNPs, as presented in Figure 3, show a characteristic intense narrow band at λmax = 400 nm and an additional band at λmax = 1000 nm. The stock solution of AgNPs with concentration of 1.9 mg/mL was used for preparation of more diluted solutions (20,40, and 60 µL of stock solution per 1 mL of water) for UV-Vis spectroscopy.  The electronic absorption spectra of the obtained AgNPs, as presented in Figure 3, show a characteristic intense narrow band at λmax = 400 nm and an additional band at λmax = 1000 nm. The stock solution of AgNPs with concentration of 1.9 mg/mL was used for preparation of more diluted solutions (20,40, and 60 µL of stock solution per 1 mL of water) for UV-Vis spectroscopy.  AgNPs were isolated from the suspension and, after drying, examined for the surface composition using the XPS method ( Figure 4). Core level spectra of Ag 3d, O 1s, and C 1s are shown in Figure 4. The collected results confirm that the stabilizer remains on the surface of the nanoparticles. This is evidenced by the peaks at E b = 285.1 ± 0.1 eV (C-C species), 286.6 ± 0.2 eV (C-OH species), and 288.7 ± 0.1 eV (carboxyl species) observed in the XPS C 1s spectra, as well as at E b = 531.5 ± 0.1 eV (O=C-O species) and 532.7 ± 0.1 eV (C-O species) in the XPS O 1s spectra [37]. In the discussed areas, we also found the features that confirm the presence of water adsorbed on the surface (E b = 535.4 eV), as well as trace amounts of K (doublet with K 2p 3/2 at 293.1 eV and K 2p 1/2 at 296.0 eV). The surface also contains silver, but its chemical state may not be uniform. Both samples show the Ag 3d 5/2 peak at 368.3 ± 0.1 eV and the Ag 3d 3/2 peak at 374.3 ± 0.1 eV. Such high binding energy value of these peaks may indicate the presence of metallic silver (oxide systems usually give peaks at E b below 368 eV) [38,39]. On the other hand, in the O 1s region, the component typical for the emission of photoelectrons from oxygen atoms bound to metal atoms (Eb = 530.2 eV) is observed. Most likely, therefore, the surface of silver is partially oxidized to form film of silver hydroxide or silver doped with oxygen atoms [40][41][42]. Notably, the presence of oxygen atoms bonded to silver was not evidenced in the case of highly biologically active silver nanoparticles prepared in regular hydrothermal conditions [31].
AgNPs were isolated from the suspension and, after drying, examined for the surface composition using the XPS method ( Figure 4). Core level spectra of Ag 3d, O 1s, and C 1s are shown in Figure 4. The collected results confirm that the stabilizer remains on the surface of the nanoparticles. This is evidenced by the peaks at Eb = 285.1 ± 0.1 eV (C-C species), 286.6 ± 0.2 eV (C-OH species), and 288.7 ± 0.1 eV (carboxyl species) observed in the XPS C 1s spectra, as well as at Eb = 531.5 ± 0.1 eV (O=C-O species) and 532.7 ± 0.1 eV (C-O species) in the XPS O 1s spectra [37]. In the discussed areas, we also found the features that confirm the presence of water adsorbed on the surface (Eb = 535.4 eV), as well as trace amounts of K (doublet with K 2p3/2 at 293.1 eV and K 2p1/2 at 296.0 eV). The surface also contains silver, but its chemical state may not be uniform. Both samples show the Ag 3d5/2 peak at 368.3 ± 0.1 eV and the Ag 3d3/2 peak at 374.3 ± 0.1 eV. Such high binding energy value of these peaks may indicate the presence of metallic silver (oxide systems usually give peaks at Eb below 368 eV) [38,39]. On the other hand, in the O 1s region, the component typical for the emission of photoelectrons from oxygen atoms bound to metal atoms (Eb = 530.2 eV) is observed. Most likely, therefore, the surface of silver is partially oxidized to form film of silver hydroxide or silver doped with oxygen atoms [40][41][42]. Notably, the presence of oxygen atoms bonded to silver was not evidenced in the case of highly biologically active silver nanoparticles prepared in regular hydrothermal conditions [31].

Preparation of Hydrogels
Inspired by our previous results in the preparation of a stable and nontoxic gold nanoparticle containing hydrogels [11] suitable for medical applications and drug delivery, we decided to use the same gelator C12Ala which had been thoroughly studied and proved to be efficient and safe [11,43,44]. The blank hydrogel containing C12Ala was prepared as a reference. At first, we measured the solubility of C12Ala in water at 20 °C. The experiments were based on a direct measurement of a weight loss of insoluble material recovered after ultrasonic-assisted dissolving of excess C12Ala in water at 30 °C, and 4 days equilibration at 20 °C without the ultrasonic irradiation. The measured solubility was determined as 116 mg/L. The development of stable hydrogels required formation of the net of fibers of gelator from the permeated solution. We found that hydrogels containing less than 5% of the gelator undergo relatively fast phase transformation and precipitation of gelator. The stable gels were obtained after rapid cooling of (prepared at 85 °C in ultrasonic bath) 7% solution of C12Ala in 0.5% aqueous solution of sodium citrate. The C12Ala is the molecule with polar and nonpolar parts. In the presence of a solvent, the gelator molecules connect with each other with the polar parts through weak hydrogen bonding

Preparation of Hydrogels
Inspired by our previous results in the preparation of a stable and nontoxic gold nanoparticle containing hydrogels [11] suitable for medical applications and drug delivery, we decided to use the same gelator C 12 Ala which had been thoroughly studied and proved to be efficient and safe [11,43,44]. The blank hydrogel containing C 12 Ala was prepared as a reference. At first, we measured the solubility of C 12 Ala in water at 20 • C. The experiments were based on a direct measurement of a weight loss of insoluble material recovered after ultrasonic-assisted dissolving of excess C 12 Ala in water at 30 • C, and 4 days equilibration at 20 • C without the ultrasonic irradiation. The measured solubility was determined as 116 mg/L. The development of stable hydrogels required formation of the net of fibers of gelator from the permeated solution. We found that hydrogels containing less than 5% of the gelator undergo relatively fast phase transformation and precipitation of gelator. The stable gels were obtained after rapid cooling of (prepared at 85 • C in ultrasonic bath) 7% solution of C 12 Ala in 0.5% aqueous solution of sodium citrate. The C 12 Ala is the molecule with polar and nonpolar parts. In the presence of a solvent, the gelator molecules connect with each other with the polar parts through weak hydrogen bonding and electrostatic interactions [44], forming thin and long fibers of the gel matrix. In the case of strongly hydrophilic molecules dissolved by polar solvents, the structures of the gel matrix look very different. ZhangPing Li and coworkers showed SEM images of the internal structure of a hydrogel made of polyethyleneimine-modified pectin, as seen in Figure 2 in [45].
The hydrogels doped with AgNPs (C 12 Ala-AgNPs) were obtained similarly from the solution of AgNPs (4.4 mg/mL and 2.2 mg/mL), sodium citrate (0.00125 M), and solid C 12 Ala. Formed hydrogels were examined by applying several physicochemical methods.

SEM Analysis
The SEM images of hydrogels stored for 5 months at 5 • C presented in Figure 5 correspond to the blank hydrogel ( Figure 5a); C 12 Ala-AgNPs containing 4 mg/L of AgNPs ( Figure 5b); AgNPs distributed among the fibers of gel, and the melted by electron beam hydrogel containing AgNPs ( Figure 5c); and separated AgNPs in completely melted gel ( Figure 5d). and electrostatic interactions [44], forming thin and long fibers of the gel matrix. In the case of strongly hydrophilic molecules dissolved by polar solvents, the structures of the gel matrix look very different. ZhangPing Li and coworkers showed SEM images of the internal structure of a hydrogel made of polyethyleneimine-modified pectin, as seen in Figure 2 in [45].
The hydrogels doped with AgNPs (C12Ala-AgNPs) were obtained similarly from the solution of AgNPs (4.4 mg/mL and 2.2 mg/mL), sodium citrate (0.00125 M), and solid C12Ala. Formed hydrogels were examined by applying several physicochemical methods.

SEM Analysis
The SEM images of hydrogels stored for 5 months at 5 °C presented in Figure 5 correspond to the blank hydrogel ( Figure    As it was measured, the average diameter of gel fibers in blank hydrogel was between d = 0.15-0.25 µm, while in hydrogel doped with silver, it was between d = 0.6-1.8 m. This could be rationalized by the assumption that the negatively charged AgNPs most strongly interact with thinner nanofibers and promote their recrystallization and fusion. The metal nanoparticles also make the hydrogel less stable under the electron beam irradiation, and the gelator fibers are melted during the measurement. We confirmed a weak interaction of AgNPs with fibers of the gelator in centrifuge experiment. The AgNPs were separated from the gel; after 15 min of rotation at 13,000 rpm, the majority of AgNPs were collected at the bottom of the centrifuge vessel (Figure 6a), and they were dissolved back after storing for 24 h at ambient temperature ( Figure 6c).
As it was measured, the average diameter of gel fibers in blank hydrogel was between d = 0.15-0.25 µm, while in hydrogel doped with silver, it was between d = 0.6-1.8 m. This could be rationalized by the assumption that the negatively charged AgNPs most strongly interact with thinner nanofibers and promote their recrystallization and fusion. The metal nanoparticles also make the hydrogel less stable under the electron beam irradiation, and the gelator fibers are melted during the measurement.
We confirmed a weak interaction of AgNPs with fibers of the gelator in centrifuge experiment. The AgNPs were separated from the gel; after 15 min of rotation at 13,000 rpm, the majority of AgNPs were collected at the bottom of the centrifuge vessel ( Figure  6a), and they were dissolved back after storing for 24 h at ambient temperature ( Figure  6c).

Thermal Resistance
As was already demonstrated, the presence of AgNPs in the liquid phase located between the nanofibers affected the properties of gel and its stability. More information about this phenomenon was gathered during thermal analysis.

The Melting and Crystallization Point of Gels
The three repetitions of the gel samples' heating and cooling process were performed in the temperature range from 20 °C to 100 °C by DSC method. Figure 7 shows the second repetition for both samples.

Thermal Resistance
As was already demonstrated, the presence of AgNPs in the liquid phase located between the nanofibers affected the properties of gel and its stability. More information about this phenomenon was gathered during thermal analysis.

The Melting and Crystallization Point of Gels
The three repetitions of the gel samples' heating and cooling process were performed in the temperature range from 20 • C to 100 • C by DSC method. Figure 7 shows the second repetition for both samples.
We confirmed a weak interaction of AgNPs with fibers of the gelator in centrifuge experiment. The AgNPs were separated from the gel; after 15 min of rotation at 13,000 rpm, the majority of AgNPs were collected at the bottom of the centrifuge vessel ( Figure  6a), and they were dissolved back after storing for 24 h at ambient temperature ( Figure  6c).

Thermal Resistance
As was already demonstrated, the presence of AgNPs in the liquid phase located between the nanofibers affected the properties of gel and its stability. More information about this phenomenon was gathered during thermal analysis.

The Melting and Crystallization Point of Gels
The three repetitions of the gel samples' heating and cooling process were performed in the temperature range from 20 °C to 100 °C by DSC method. Figure 7 shows the second repetition for both samples.  chemical characteristics in the multicortical dissolution and gelling process. Moreover, the presence of silver nanoparticles does not significantly affect the stability of the gel matrix.

Temperature Decomposition of Gels
The total decomposition of the gels was recorded at a temperature of about 350 • C. In comparison, the total decomposition temperature of analogical gel enriched with gold nanoparticles (C 12 Ala-AuNPs) was about 300 • C (see Figure 2 in [11]). Figure 8 shows thermograms for C 12 Ala gel and C 12 Ala-AgNPs gel samples, obtained for a heating rate of 10 • C/min. one degree between the pure sample C12Ala gel and the sample doped with silve particles, C12Ala-AgNPs. The crystallization point of the sample does not depend nanoparticle content and amounts to 35 °C. The results of the DSC test indicate t gel samples are stable in the tested temperature range; they do not change their ch characteristics in the multicortical dissolution and gelling process. Moreover, the p of silver nanoparticles does not significantly affect the stability of the gel matrix.

Temperature Decomposition of Gels
The total decomposition of the gels was recorded at a temperature of about In comparison, the total decomposition temperature of analogical gel enriched wi nanoparticles (C12Ala-AuNPs) was about 300 °C (see Figure 2 in [11]). Figure 8 show mograms for C12Ala gel and C12Ala-AgNPs gel samples, obtained for a heating ra °C/min. As can be seen in Figure 8, the very fast weight loss (from 100% to ~10% of w was recorded for both samples in the temperature range from 20 °C to 125 °C. This is related to the rapid evaporation of the solvent from the gels. In the temperatur from 125 °C to 275 °C for both samples, another process of a mass loss occurs, rel the decomposition of the gelator C12Ala. Moreover, as shown in the graph of th derivative (Figure 9), over the temperature range of 330-350 °C, an additional clearly visible. This peak is related to the degradation of the silver particles (AgN suggests that the silver nanoparticles are not chemically bound to the C12Ala gelat ecules. In the case of strong bonding of nanoparticles to gelator fibers, the decomp peak for nanoparticles would not be so pronounced; nanoparticles would decomp gether with gelator fibers. The TGA measurements were performed with heating 1 °C/min, 5 °C/min, and 10 °C/min to calculate the kinetics of samples decomposi the Ozawa-Flynn-Wall (OFW) theory [46]. The results (not shown in this work) we ilar to the sample enriched with gold nanoparticles AuNPs. Within the limit of 10% phase loss, we found that C12Ala-AgNPs can stay at a temperature of 10 °C for a min, whereas increasing the temperature to 90 °C shortens this time to only a few m For C12Ala-AuNPs, the limit of 10% of weight at 10 °C was reached after 70 min [1 As can be seen in Figure 8, the very fast weight loss (from 100% to~10% of weight) was recorded for both samples in the temperature range from 20 • C to 125 • C. This process is related to the rapid evaporation of the solvent from the gels. In the temperature range from 125 • C to 275 • C for both samples, another process of a mass loss occurs, related to the decomposition of the gelator C 12 Ala. Moreover, as shown in the graph of the TGA derivative (Figure 9), over the temperature range of 330-350 • C, an additional peak is clearly visible. This peak is related to the degradation of the silver particles (AgNPs) and suggests that the silver nanoparticles are not chemically bound to the C 12 Ala gelator molecules. In the case of strong bonding of nanoparticles to gelator fibers, the decomposition peak for nanoparticles would not be so pronounced; nanoparticles would decompose together with gelator fibers. The TGA measurements were performed with heating rates of 1 • C/min, 5 • C/min, and 10 • C/min to calculate the kinetics of samples decomposition by the Ozawa-Flynn-Wall (OFW) theory [46]. The results (not shown in this work) were similar to the sample enriched with gold nanoparticles AuNPs. Within the limit of 10% liquid phase loss, we found that C 12 Ala-AgNPs can stay at a temperature of 10 • C for about 65 min, whereas increasing the temperature to 90 • C shortens this time to only a few minutes. For C 12 Ala-AuNPs, the limit of 10% of weight at 10 • C was reached after 70 min [11]. In general, the thermal analysis proves the stability of hydrogels at ambient temper ature and the lack of strong interaction between AgNPs and C12Ala gelator.

Antimicrobial Properties
In the context of the biological activity of silver, the antimicrobial properties of the metal are the most common. Newly synthesized at low temperature AgNPs were exam ined by the broth microdilution method against twelve bacteria and one fungal strains Surprisingly, the AgNPs at the tested concentration of up to 1 mg/mL did not inhibit the growth of any of the tested microorganisms, neither bacteria nor fungi ( Table 1). The re sults are in opposition to these presented by others, where AgNPs were obtained in the hydrothermal synthesis. Hwang et al. also tested antibacterial activity of AgNPs agains human pathogenic bacteria, including two strains of E. coli and P. aeruginosa, S. aureus Nanoparticles showed antibacterial activity with MIC (minimal inhibitory concentration values of 0.5-2 µg/mL [20]. In research by Pucelik et al. on multifunctional silver nanopar ticles modified with 11-mercapto-N, N, N-trimethylammonium chloride (TMA), and so dium citrate (TSC), MIC values of 0.17 µg/mL and 0.05 µg/mL, respectively, for E. coli and S. aureus were obtained [31]. AgNPs were also the subject of the research of Loo et al. [47] In their study, the MICs of AgNPs against E. coli, K. pneumoniae, S. typhimurium, and S enteritidis were 7.8, 3.9, 3.9, and 3.9 µg/mL, respectively. In antimicrobial tests performed by Liao et al., AgNPs were shown to have a strong bactericidal effect on drug-resistan and multidrug-resistant P. aeruginosa with an MIC range of 1.4-5.6 µg/mL [48]. Antimi crobial studies on the gelator C12Ala and its variant containing AgNPs showed a lack o both antibacterial and antifungal properties (Table 1).
In addition to antimicrobial properties, silver nanoparticles are known for their anti cancer activity. The synthesized AgNPs have been tested for anticancer activity agains normal (CCD-11Lu) and cancer (HeLa, SW480) human cell lines. At the lowest tested con centration of 0.5 µg/mL against HeLa, SW480, and CCD cells, cell viability was very close or equal, to 100%. However, at the highest concentration (220 µg/mL) for HeLa cell line AgNPs inhibit the proliferation only by 5.73% after 24 h of incubation and by 7.41% after 48 h. In the case of the SW480 and CCD-11Lu lines, the inhibition of proliferation was higher and amounted to 23.54% and 20.5% after 48 h of incubation, respectively ( Figure  10). In general, the thermal analysis proves the stability of hydrogels at ambient temperature and the lack of strong interaction between AgNPs and C 12 Ala gelator.

Antimicrobial Properties
In the context of the biological activity of silver, the antimicrobial properties of the metal are the most common. Newly synthesized at low temperature AgNPs were examined by the broth microdilution method against twelve bacteria and one fungal strains. Surprisingly, the AgNPs at the tested concentration of up to 1 mg/mL did not inhibit the growth of any of the tested microorganisms, neither bacteria nor fungi ( Table 1). The results are in opposition to these presented by others, where AgNPs were obtained in the hydrothermal synthesis. Hwang et al. also tested antibacterial activity of AgNPs against human pathogenic bacteria, including two strains of E. coli and P. aeruginosa, S. aureus. Nanoparticles showed antibacterial activity with MIC (minimal inhibitory concentration) values of 0.5-2 µg/mL [20]. In research by Pucelik et al. on multifunctional silver nanoparticles modified with 11-mercapto-N, N, N-trimethylammonium chloride (TMA), and sodium citrate (TSC), MIC values of 0.17 µg/mL and 0.05 µg/mL, respectively, for E. coli and S. aureus were obtained [31]. AgNPs were also the subject of the research of Loo et al. [47]. In their study, the MICs of AgNPs against E. coli, K. pneumoniae, S. typhimurium, and S. enteritidis were 7.8, 3.9, 3.9, and 3.9 µg/mL, respectively. In antimicrobial tests performed by Liao et al., AgNPs were shown to have a strong bactericidal effect on drug-resistant and multidrug-resistant P. aeruginosa with an MIC range of 1.4-5.6 µg/mL [48]. Antimicrobial studies on the gelator C 12 Ala and its variant containing AgNPs showed a lack of both antibacterial and antifungal properties (Table 1). Table 1. Assessment of antibacterial and antifungal properties of AgNPs, and C 12 Ala, as well as C 12 Ala-AgNPs, gels. MIC values expressed in µg/mL are presented. Chloramphenicol (CPL) and Amphotericin B (AmpB) were used as control antibacterial and antifungal agents, respectively. In addition to antimicrobial properties, silver nanoparticles are known for their anticancer activity. The synthesized AgNPs have been tested for anticancer activity against normal (CCD-11Lu) and cancer (HeLa, SW480) human cell lines. At the lowest tested concentration of 0.5 µg/mL against HeLa, SW480, and CCD cells, cell viability was very close, or equal, to 100%. However, at the highest concentration (220 µg/mL) for HeLa cell line, AgNPs inhibit the proliferation only by 5.73% after 24 h of incubation and by 7.41% after 48 h. In the case of the SW480 and CCD-11Lu lines, the inhibition of proliferation was higher and amounted to 23.54% and 20.5% after 48 h of incubation, respectively ( Figure 10).

Hemolytic Properties
In order to confirm the low toxicity of metal nanoparticles against normal human cells, AgNPs alone, as well as in the combination with the gelator, were tested for hemolytic activity using human erythrocytes (Figure 11). At the concentration of 11 µg/mL, the nanoparticles do not cause hemolysis of the blood cells. In turn, at the concentrations of 22 and 110 µg/mL, 4.2% and 8.2% of the blood cells were lysed, respectively. The highest percentage of hemolysis (11%) was obtained at the highest concentration (220 µg/mL). The results show that the AgNPs, even at high concentration, have little hemolytic activity. Korolev et al. [51] and Zharkova and team [52] obtained similar results. They found that Similarly to antimicrobial inactivity, the AgNPs show the minor influence on human cancer cells only at the highest tested concentration, which does not correspond with the results obtained by others, where hydrothermal AgNPs synthesis was applied. Pucelik et al. found that AgNPs are highly toxic to cancer cells [31]. The studies included AgNPs of different sizes (DLS: 3.1-41 nm) with positive surface charge: Ag@TMA1, Ag@TMA2, and negative surface charge: Ag@TSC1, Ag@TSC2 against human keratinocytes (Ha-CaT) and cancer cell line: CT26, 4T1. The test included the concentration of 0.1 and 0.5 µg/mL and incubations for 2 and 24 h. In concentration of 0.50 µg/mL, AgNPs show high toxicity in all tested cases. Other studies on the cytotoxicity of AgNPs were carried out against breast cancer cell lines (MCF-7) and human lung fibroblast cell lines (WI38). The IC 50 of cellular inhibition of silver nanoparticles was observed at 27.79 ± 2.3 and 31.78 ± 2.2 µg/mL, respectively [49]. On the other hand, studies on biosynthesized silver nanoparticles showed reduced cell viability in colon cancer cells (HCT-116) at an IC 50 concentration of 100 µg/mL [50]. Next, the gelator alone, as well as in the combination with AgNPs, was tested against two cancer and one nontumor human cell lines. The presented high IC 50 values, starting from 1.86 mg/mL revealed low anticancer activity of these substances ( Table 2). In spite of such results, firstly, nontumor CCD-11Lu cells showed lower susceptibility to gelators, and, secondly, addition of AgNPs resulted in higher cytotoxicity, especially against tumor SW480 cell line.

Hemolytic Properties
In order to confirm the low toxicity of metal nanoparticles against normal human cells, AgNPs alone, as well as in the combination with the gelator, were tested for hemolytic activity using human erythrocytes (Figure 11). At the concentration of 11 µg/mL, the nanoparticles do not cause hemolysis of the blood cells. In turn, at the concentrations of 22 and 110 µg/mL, 4.2% and 8.2% of the blood cells were lysed, respectively. The highest percentage of hemolysis (11%) was obtained at the highest concentration (220 µg/mL). The results show that the AgNPs, even at high concentration, have little hemolytic activity. Korolev et al. [51] and Zharkova and team [52] obtained similar results. They found that the hemolytic activity of unmodified AgNPs was minimal and did not exceed a few percent. In turn, Chen et al. [53] investigated the hemolytic activity against three diameters of AgNPs. Studies showed that AgNPs15 resulted in a much higher level hemolysis (60%) compared to AgNPs50 and AgNPs100, which caused less than 12% hemolysis even at the highest tested concentration. The combination of AgNPs with the gelator results in slightly higher hemolysis in comparison with an activity of sole C 12 Ala, but taking into consideration that gels were tested at quite high concentrations, this effect was rather irrelevant (Figure 11).

Ecotoxic Properties
In the final stage, silver nanoparticles and gelators were tested for ecotoxic properties using the in vivo Danio rerio model (Figure 12).

Ecotoxic Properties
In the final stage, silver nanoparticles and gelators were tested for ecotoxic properties using the in vivo Danio rerio model ( Figure 12). Figure 11. Hemolytic activity of AgNPs and gelators measured by percent of lysed erythrocytes compared to control (Triton X-100). (a) AgNPs; (b) C12Ala; (c) C12Ala-AgNPs.

Ecotoxic Properties
In the final stage, silver nanoparticles and gelators were tested for ecotoxic properties using the in vivo Danio rerio model (Figure 12).  C 12 Ala-AgNPs was not toxic at all, while compounds AgNPs and C 12 Ala were toxic at the dose of 5 mg/mL. No malformations were observed. The toxicity of AgNPs and C 12 Ala were exerted in coagulation of fertilized eggs in concentrations of 5 mg/mL and higher.

General CPL
AmpB, TSC, silver nitrate, tannic acid, and PEI (branched, analytical standard) were purchased from Sigma-Aldrich Chemicals, St. Louis, MO, USA. Distilled water was obtained with Millipore system (ρ = 18.2 MΩ) and used in all experiments and for washing glass parts of the laboratory equipment. Silicon wafers used in the experiments were purchased from Siegert Wafer GmbH (Aachen, Germany). XPS measurements were performed in a Prevac photoelectron spectrometer consisting of an analysis UHV chamber with a hemispherical analyzer (VG SCIENTA R3000 (Pleasanton, CA, USA)). A monochromatized aluminum source Al Kα (hν = 1486.6 eV) was used for acquiring survey-and cor-level spectra. The scale of binding energy value was calibrated by referring to a position of Au 4f (E b = 84.0 eV). Curve-fitting analysis of all spectra was performed in the Casa XPS software using the mixed Gauss and Lorentz function (GL = 30) after subtraction of the The measurements were conducted using appropriate quartz cuvettes, dedicated to such measurements. The analysis of the statistical distribution of the nanoparticles' sizes was carried out through computing SEM images. To evaluate the NPs size distribution, an analysis software for graphical images was implemented: ImageJ (https://imagej.nih.gov/, accessed on 26 December 2022). The statistical analysis was conducted for a probe of N = 500. UV-Vis spectroscopy was implemented to examine the solutions of manufactured nanoparticles in the wavelength range of 300-1100 nm, using a UV-2600 spectrometer (Shimadzu, Kyoto, Japan). The measurements were conducted using appropriate quartz cuvettes, dedicated to such measurements. The weight concentration of silver (Ag) nanoparticles was measured by a densitometer DMA 5000M from Anton Paar. The SEM measurements were recorded on a ZEISS Ultra Plus microscope.

AgNPs Preparation
Silver nanoparticles with controlled dimensions and surface properties were obtained by a modified method published in our previous work [31]. A total of 20 mL of 25 mM solution of TSC was mixed with 2 mL 5 mM solution of tannic acid and diluted with 78 mL of water. The obtained solution was stirred for 15 min at room temperature (RT), then 3 mL of 25 mM solution of AgNO 3 was added dropwise. The change in the color of the solution, from bright yellow through intensive yellow to slightly red, within several minutes indicated the formation of AgNPs coated with the citric ligands. After the reaction, the final solution was purified by recentrifugation at 2500 rcf, which led to the separation of NPs larger than 40 nm from the supernatant. The purification process was carried out by recentrifugation at 18,000 rcf and then the solution was washed several times, resulting in a precipitate of AgNPs with water. The size and zeta potential of the final AgNPs were estimated by DLS and SEM. The concentration of the obtained suspension was determined by density measurement, which was 4.4 mg/L.

Determination of Concentration of AgNPs
The weight concentration of silver (Ag) nanoparticles in the solution after purification was evaluated by measuring the density of the native suspension ρ s and the effluent ρ e obtained following centrifugation. The mass concentration is then determined using the formula [54]: where: ρ p = 10.49 g/cm 3 is the specific density of silver nanoparticles [55]. According to the discussed procedure, the concentration of AgNPs was found to be 4.4 mg/L.

Silicon Substrate Treatment for NPs Microscopy Observations
The procedure is based on thoroughly washing the silicon substrate (1 cm × 1 cm) in methanol and then in ultrapure water under sonication treatment. In the next step, ultraclean and dried under argon flush substrates were oxidized by piranha solution (3 parts of concentrated sulfuric acid and 1 part of 30% hydrogen peroxide solution; 15 min). The PEI polyelectrolyte monolayer was applied onto the surface of the silicon substrate by the layer-by-layer LBL technique. In the case of the negative charge of NPs, one PEI layer was formed on the surface, as a result of immersing substrates in a PEI solution (1 mg/mL; 30 min). The deposition of the NPs was carried out by immersing the substrates in the nanoparticles' dispersion during 20 min. After this process, the substrates were thoroughly washed with water and dried with argon. Freshly prepared solutions of polyelectrolytes, which were previously sonicated, were used.

Preparation of the Hydrogels, Typical Procedure
The dry glass vial equipped with the stirrer magnet was charged with 7.3 mL of solution AgNPs (4.4 mg/mL), 560 mg of solid C 12 Ala was added, and after 2 min of stirring, 0.12 mL of a 1.25 M solution TSC was added. The vial was closed and the reaction mixture was heated at 85-90 • C in ultrasonic bath for 10 min to achieve the homogenous mixture. Next, the vial was cooled down to 0-5 • C in an ice bath without stirring. After the cooling was completed, the stable at ambient (and lower) temperature light yellow gel was formed, as presented in Figure 5B.

Differential Scanning Calorimetry (DSC)
DSC measurement was used to analyze phase transitions related to temperature change in samples and determine the phase and structural changes taking place in the sample during heating along with their kinetics, exothermic and endothermic chemical reactions, changes in the heat capacity of the sample, and, in some cases, as well as the temperature stability of the samples.

Thermal Gravimetric Analysis (TGA)
TGA was used to record changes in the mass of a sample during its thermal decomposition to make conclusions regarding the amount of thermal transformation and the temperature at which this transformation takes place.

Determination of Minimum Inhibitory Concentrations (MICs)
The substances were investigated in vitro for antimicrobial activities. In these studies, the broth microdilution was used. The MIC of the substances was evaluated by the microdilution broth method in 96-well polystyrene plates. The tests were performed in accordance with the guidelines of the European Committee on Antimicrobial Susceptibility Testing (EUCAST) [56] and for fungi were performed. The final concentrations of AgNPs ranged from 1000 µg/mL to 0.35 µg/mL, C 12 Ala ranged from 6000 µg/mL to 11.7 µg/mL, and C 12 Ala + AgNPs ranged from 6000 µg/mL to 11.7 µg/mL. Bacterial and fungal suspensions were prepared in sterile NaCl with an optical density of 0.5 McFarland standard. Next, the microbial suspension was introduced into each well of the microplate containing broth and various concentrations of the tested substances. After 24 h incubation, the MIC value was assessed visually as the minimal concentration of the samples that showed complete microbial growth inhibition. Each concentration range for all microbial species was tested in triplicate. Appropriate DMSO, sterile, and growth controls were performed. The media with and without tested substances/DMSO were used as controls. Standard antibiotics, antibacterial CPL, and antifungal AmpB were used as reference substances.

Antiproliferative Assay
For antiproliferative assay, cells of each line were seeded in 96-well microplates (Wuxi Nest Biotechnology, Wuxi, Jiangsu, China) at a density of 2.5 × 10 4 cells/mL in 100 µL DMEM + GlutaMAX supplemented with 10% heat-inactivated FBS in two sets for different periods of tested compound exposure. After 24 h of cell attachment, plates were washed with 100 µL/well of Dulbecco's phosphate-buffered saline (DPBS) and the cells were treated with increasing concentrations (0.0005-0.22 mg/mL final concentration) of AgNPs and 0.056-100 mg/mL final concentration of C 12 Ala and C 12 Ala-AgNPs prepared in fresh FBSfree medium for 24 and 48 h. All stock solutions were diluted to the desired concentration with the culture medium only. Each concentration was tested in triplicate. Cytotoxicity of compounds was assessed using (3-[4,5-dimethylthiazol-2-yl])-2,5 diphenyl tetrazolium bromide (MTT) assay as described below. Following 24 and 48 h of compound exposure, control medium or test exposures medium were removed, the cells were rinsed with DPBS, 100 µL of fresh medium (without FBS or antibiotics) containing 0.5 mg/mL of MTT was added to each well, and the plates were incubated for 3 h at 37 • C in a 5% CO 2 humidified incubator. After the incubation period, the medium was discarded, the cells were washed with 100 µL of DPBS, and 100 µL of DMSO was added to each well to extract the dye. The plate was shaken for 10 min and the absorbance was measured at 570 nm. Viability was calculated as the ratio of the mean of OD obtained for each condition to the control condition. Calculations of IC 50 values and statistical analysis were performed in GraphPad Prism 9 software.

Hemolytic Activity
The hemolytic activity of the AgNPs and gelators was determined on human red blood cells. Human erythrocytes were harvested by centrifugation for 10 min at 2000 rpm and 4 • C. Then, the pellets were washed in PBS buffer (10 mM phosphate, pH 7.5; 150 mM NaCl). This step was performed three times. The resulting suspension was serially diluted 10-fold in PBS. A further 1:10 dilution of PBS was prepared from this suspension. Then, 450 µL of the final diluted erythrocytes were added to microcentrifuge tubes, which contained test compounds in an amount of 50 µL each. The final concentrations was 11-220 µg/mL (AgNPs), and 0.1-10 mg/mL (C 12 Ala and C 12 Ala + AgNPs). Test concentrations were prepared by dissolving in PBS, and 1% Triton was used as a positive control, causing total hemolysis. The tubes were incubated at 37 • C for 1 h and then centrifuged for 10 min at 2000 rpm and 4 • C. A total of 150 µL of each tube was transferred to a flat-bottomed microtiter plate. The absorbance was measured at 450 nm. The hemolysis percentage was calculated by the following equation: % hemolysis = (A 450 of test compound treated sample − A 450 of buffer treated sample/ A 450 of 1% Triton X-100 treated sample − A 450 of buffer treated sample) × 100%. The experiments were performed in duplicate.

Ecotoxicity
To determine the toxicity of AgNPs, C 12 Ala, and C 12 Ala-AgNPs, the FET test was performed on zebra-fish (Danio rerio) according to OECD Test Guideline 236. Briefly, newly fertilized zebra-fish eggs were exposed to solutions of compounds for a period of 96 h at concentrations ranging from 1 to 10 mg/mL. The system applied in the experiment was static, as the changes of solution concentrations did not exceed the range of 20% of nominal concentration values.
The E3 solution (5 mmol/L NaCl, 0.17 mmol/L KCl, 0.33 mmol/L CaCl 2 , and 0.33 mmol/L MgSO 4 , containing no methylene blue, with a pH value of about 7.2) was used as embryo culture medium as well as to prepare the solutions. The experiment was performed in 24-well plates, with five embryos per well, ten per group, in three repetitions. Each plate was covered and kept in an incubator set at 28 ± 0.5 • C under a light/dark period of 12/12 h. At the end of the exposure period (96 hours post fertilization (hpf)), acute toxicity was determined based on a positive outcome in any of the four visual indicators of lethality, including the coagulation of fertilized eggs, lack of somite formation, lack of detachment of the tailbud from the yolk sac, and lack of heartbeat. The value of EC 50 was calculated.

Conclusions
The main goal of this work was to prepare and investigate the properties of a new C 12 Ala-based hydrogel enriched with AgNPs in terms of its suitability for pharmaceutical purposes. On the basis of physical and biological tests, it was found that silver nanoparticles do not disturb the stability of the gel matrix, and both matrixes, pure and silver-enriched are stable in the temperature range of 20 • C to 100 • C. No interactions were found between gelator molecules and silver nanoparticles, which diffuse freely in the pores filled with the liquid phase of hydrogel.
In comparison with the biological activity of AgNPs published elsewhere, our nanoparticles show high level of biological neutrality when tested against microorganisms, human cells as well as zebra-fish embryos. Combination of AgNPs with the gelator C 12 Ala studied in parallel also showed trace biological activity towards the used models. Such biologically neutral assembly may be taken into consideration as promising agent for applications where side effects are unwanted, e.g., in drug delivery.